Electrochemical fabrication and characterization of poly (o-phenylenediamine) nanotubes by template method
Indian Journal of ChemistryVol. 48A, February 2009, pp. 198-201 Electrochemical fabrication and derivative which can be achieved through substitutingcharacterization of poly(o-phenylenediamine) hydrogens by an amino group in an aniline nucleus. PoPD is usually prepared by electrochemical nanotubes by template method polymerization. The PoPD obtained by this method usually has an irregular morphology as compared to T Maiyalagan & B Viswanathan* that obtained by the conventional polymerizationNational Centre for Catalysis Research, Department of Chemistry, method. The detailed synthetic procedure of the Indian Institute of Technology Madras, Chennai 600 036, India template-synthesized poly (o-phenylenediamine) Email: firstname.lastname@example.org nanotube on Nafion and graphite are shown Received 20 October 2008; revised 9 January 2009 schematically in Fig. 1. The conventional synthesis of poly (o-phenylenediamine) was carried out in the The fabrication of conducting poly (o-phenylenediamine) same way without the alumina membrane as thenanotube by electropolymerisation on alumina wafers (Whatman template.Anodisc 47 filter disk) is described. The nanotubes have beencharacterized by FTIR, UV-vis, SEM, TEM and AFM studies. PoPD nanobelts can be synthesized from anSEM and TEM results reveal that the polymer nanotubes have o-phenylenediamine (oPD)-HAuCl4 or oPD-AgNO3uniform and well-aligned arrays and their diameter and length aqueous solution at room temperature without usingmatch with the aspect ratios of the anodisc aluminium oxide any surfactant20,21. However, the resulting precipitates(AAO) membrane. are not “pure”, and there are some Au or Ag particleKeywords:Conducting polymers, Electropolymerization, byproducts, and therefore a post-separation Nanomaterials, Nanotube arrays, Template method, process should be involved to obtain the pure 1D Poly o-phenylenediamine structure. Herein, we report the preparation of PoPDIPC Code: Int. Cl.8 B82B1/00; C08G73/00; C25B3/02 nanotubes with uniform length and diameter using template assisted electrochemical synthesis. In thisIn recent years, one-dimensional nanostructures method the oxidizing agents, surfactants have notincluding nanofibers, nanotubes, nanorods and used and therefore, the obtained PoPD nanotube isnanobelts of conducting polymers have been studied “pure”.extensively. These 1D nanostructured materialshave distinct geometries, and novel physical Experimentaland chemical properties, which are probably The present study was carried out in aqueousapplicable in nanodevices1. There are many solutions. Purified water obtained by passing distilledmethods to be developed for synthesizing 1D water through a milli Q (Millipore) water purificationconducting polymers, for example, a hard- system was used as solvent. o-Phenylenediaminetemplate based method to prepare 1D conducting (o-PD) was purchased from Aldrich. Sulphuric acidpolymers has been reported2-4. Micelles, surfactants,liquid crystals, thiolated cyclodextrins andpolyacids have also been used as a soft-template toprepare nanofibers and nanotubes of conductingpolymers5-11. The template synthesis method has been widelyused for preparing nanostructured materials, whichinvolves the synthesis of the desired material withinthe pores of a membrane to generate nanotubes ofcylindrical nature with uniform diameter12-19. Fig. 1—Template assisted electrochemical synthesis ofPoly (o-phenylenediamine) (PoPD) is a polyaniline conducting polymer nanotube.
NOTES 199was obtained from Fischer Chemicals. Nafion repeatedly washed with deionized water to remove the(5 wt %) solution was obtained from Dupont and used residual NaOH. It was subsequently immersed in 1%as received. Anodisc aluminium oxide (AAO) HBF4 for 10 minutes and then washed with deionizedmembranes were obtained from Whatman Anopore water again. The composite after the dissolution of theFilters. template was designated as graphite/Naf/PoPDTemp. All experiments were carried out in a conventional The schematic view of the homemade electrochemicalone-compartment cell with a Pt counter electrode and cell for the preparation of template-synthesizeda saturated calomel reference electrode, at room poly (o-phenylenediamine) nanotube is shown intemperature. First, the graphite electrode was coated Fig. 2.with Nafion solution and the membrane is hot pressed The scanning electron micrographs were obtainedwith the graphite. Nafion not only acts as a binder but using JEOL instrument (model JSM-840), working atalso provides both ionic and electronic contact and 15 keV. The nanotubes were sonicated in acetone forfavours proton transport. Then the graphite electrode 20 minutes and then were dropped on the cleaned Siwas used as current collector and contacted with the substrates. The AFM imaging was performed in airtemplate membrane. The membrane together with the using the Nanoscope IIIA atomic force microscopecurrent collector was fixed between two teflon rings. (Digital Instruments, St. Barbara, CA) operated inThe area of the membrane contacted to the electrode contact mode. For transmission electron microscopicwas ca. 1 cm2. The solution was de-aerated by studies, the nanotubes dispersed in ethanol werebubbling dry nitrogen gas for 15 min before placed on the copper grid and the images wereelectrochemical polymerization. The electropolymeri- obtained using Phillips Instrument (model 420),zation of o-Phenylenediamine (o-PD) was carried out operating at 120 keV. The IR spectrum was recordedwith a BAS 100B Electrochemical Workstation with Perkin-Elmer (L-710) spectrophotometer.(Bioanalytical Systems Inc., West Lafayette, IN). Thepoly o-phenylenediamine nanotubes were grown Results and discussionpotentiodymanically between -0.2 V and 1.2 V The electropolymerisation of o-Phenylenediaminecontaining 5 mM oPD. The length of the nanotubes (oPD) monomer on the alumina template was carriedwas controlled by the total charges passed in the cell. out by cyclic voltammetry was shown in Fig. 3. A The alumina membrane from broad anodic peak is been in the potential range fromgraphite/Naf/PoPDTemp was removed by immersingthe composite in 0.1 M NaOH for 15 minutes. Thecomposite after the dissolution of the template wasFig. 2—Schematic view of an electrochemical cell for theformation of nanostructured materials. [RE, reference electrode; Fig. 3—Cyclic voltammograms showing the polymerization ofAE, auxiliary electrode; WE, working electrode (template 0.5 M o-phenylenediamine in 0.5 M H2SO4 solution. [(Scan rate:membrane with a deposited Nation contact layer)]. 50 mVs−1)].
200 INDIAN J CHEM, SEC A, FEBRUARY 2009Fig. 4—(a) SEM images of conventionally synthesized PoPD polymer; (b-c) SEM images of template synthesized PoPD polymernanotubes; (d) AFM image of PoPD polymer nanotubes.+0.2 V to 1.2 V, which indicates an oxidative process characteristic of the substitution pattern on theof o-PD. In all the cases no reduction peak is found in aromatic ring. The band at 812 cm−1 may be assignedthe reverse scans, thus suggesting that the oxidized to the vibration of the 1,4-disubstituded ring22. TheoPD is involved in further chemical processes leading intense band at 1450 cm−1 is attributed to the C=Nto non-reducible species in the potential range stretching vibration. This suggests that a considerableadopted. portion of C=N bond existed in the PoPD nanotubes. The UV-vis absorption spectra of the It can be noted that the presence of this band in thepoly (o-phenylenediamine) (PoPD) nanotubes were PoPD backbone indicates that the polymer chain hasstudied. A single, large absorption band around an extensive π conjugation between polymer chain364.3 nm is seen in the UV-vis spectra of PoPD. The and all nitrogen atoms. This is consistent withband is due to inter-band charge transfer associated the results of UV-vis spectroscopy andwith excitation of benzenoid to quinoid moieties electrochemical experiments. Also the results of FTIR(optical absorption of the metallic polar on band of spectra of PoPD nanotubes agree well with previousthe conducting form). reports23-25. The FT-IR spectroscopy was used to identify the The SEM image of the conventionally synthesizedstructure of the PoPD. The absorption band in the conducting poly (o-phenylenediamine) is shown inFT-IR spectra of PoPD appears around 3400 cm−1, Fig. 4a. The image shows ladder morphology and acorresponding to the N-H stretching vibration. The dense coverage of poly (o-phenylenediamine) onabsorption bands in the 650-900 cm−1 region are graphite, which are not uniform in nature.
NOTES 201 It is evident from Fig. 4b that the uniform, 5 Qiu H J & Wan X, J Polym Sci Part A Polym Chem, 39cylindrical, monodispersed nanotubes of PoPD after (2001) 3485. 6 Wei Z X, Zhang Z M & Wan M X, Langmuir, 18 (2002)the removal of the template project perpendicularly to 917.the graphite. The open ends of the uniform nanotube 7 Michaelson J C & McEvoy A J, Chem Commun, 1 (1994) 79.are clearly seen in this image. Figure 4c shows the 8 Huang L M, Wang Z B, Wang H T, Cheng X L, Mitra A &picture of the conducting polymeric tubules taken at a Yan Y X, J Mater Chem, 12 (2002) 388.tilted angle, in a different region. It is evident from 9 Choi S J & Park S M, Adv Mater, 12 (2000) 1547.the image that the density of nanotubes is quite high, 10 Liu J M & Yang S C, Chem Commun, 21 (1991) 1529. 11 Lu X, Yu Y, Chen L, Mao H, Wang L, Zhang W & Wei Y,in all the regions. These tubes are uniformly Polymer, 46 (2005) 5329.distributed in a regular array on the graphite with an 12 Martin C R, Science, 266 (1994) 1961.outer diameter (200 nm) that almost matches the pore 13 Maiyalagan T, Viswanathan B & Varadaraju U V, Bulldiameter of the template. Mater Sci, 29 (2006) 705. AFM images of the synthesized poly 14 Maiyalagan T & Viswanathan B, Mater Chem Phys, 93(o-phenylenediamine) nanotubes deposited on a (2005) 291. 15 Maiyalagan T & Viswanathan B, Indian J Chem, 45A (2006)silicon substrate were also studied and shown in 839.Fig. 4(d). The AFM tip was carefully scanned across 16 Maiyalagan T, Appl Catal B Environ, 89 (2008) 286.the tube surface in a direction perpendicular to the 17 Maiyalagan T, Viswanathan B & Varadaraju U V, J Nanoscitube axis. AFM image shows the bunch of polymer Nanotechnol, 6 (2006) 2067.nanotube on the silicon substrate further confirming 18 Maiyalagan T & Viswanathan B, J Power Sourc, 175 (2008)the electropolymerization of o-phenylenediamine. A 789. 19 Maiyalagan T, Viswanathan B & Varadaraju U V,probable reason for this is that the polymerization Electrochem Commun, 7 (2005) 905.inside the confined space of the pores, combined with 20 Sun X , Dong S & Wang E , Macromol Rapid Commun, 26electrostatic interaction, ensures the alignment of the (2005) 1504.resulting polymers on the walls of the pores of the 21 Sun X P, Dong S J & Wang E K, Chem Commun,template26. (2004)1182. 22 Guay J & Dao L H, J Electroanal Chem, 274 (1989) 135. 23 Jiang H Q, Sun X P, Huang M H, Wang Y L, Li D & Dong SReferences J, Langmuir, 22 (2006) 3358.1 Long Y, Chen Z, Wang N, Ma Y, Zhang Z, Zhang L & Wan 24 Ichinohe D, Saitoh N & Kise H, Macromol Chem Phys, 199 M, App Phys Lett, 83 (2003) 1863. (1998) 1241.2 Wu C G & Bein T Science, 264 (1994) 1757. 25 Ichinohe D, Muranaka T, Sasaki T, Kobayashi M & Kise H,3 Parthasarathy R V & Martin C R, Chem Mater, 6 (1994) J Polym Sci Part A Polym Chem, 36 (1998) 2593. 1627.4 Wang C W, Wang Z, Li M K & Li H L, Chem Phys Lett, 341 26 Sommerdijk N A J M, Nolte R J M & Kros A, Adv Mater, 23 (2001) 431. (2002) 1779.